Theoretical Study of Specific Heat and Density of States of MgB_{2} Superconductor in Two Band Model ()

Anuj Nuwal, Shyam Lal Kakani

Department of Physics, Sangam University, Bhilwara, India.

Shastri Nagar, New Housing Board, Bhilwara, India.

**DOI: **10.4236/wjcmp.2013.31006
PDF
HTML XML
5,277
Downloads
8,573
Views
Citations

Department of Physics, Sangam University, Bhilwara, India.

Shastri Nagar, New Housing Board, Bhilwara, India.

MgB_{2} with *T _{c}* ≈ 40 K, is a record-breaking compound among the s-p metals and alloys. It appears that this material is a rare example of the two band electronic structures, which are weakly connected with each other. Experimental results clearly reveal that boron sub-lattice conduction band is mainly responsible for superconductivity in this simple compound. Experiments such as tunneling spectroscopy, specific heat measurements, and high resolution spectroscopy show that there are two superconducting gaps. Considering a canonical two band BCS Hamiltonian containing a Fermi Surface of π- and

Share and Cite:

Nuwal, A. and Kakani, S. (2013) Theoretical Study of Specific Heat and Density of States of MgB_{2} Superconductor in Two Band Model. *World Journal of Condensed Matter Physics*, **3**, 33-42. doi: 10.4236/wjcmp.2013.31006.

1. Introduction

The surprising discovery of superconductivity in the novel system MgB_{2} with T_{c} = 39 K by Nagamatsu et al. [1] has stimulated new excitement in condensed matter physics. This discovery certainly revived the interest in the field of superconductivity especially in non-oxides, and initiated a search for superconductivity in related boron compounds [2]. Its high critical temperature gives hope for obtaining even higher T_{c} for similar compounds.

The crystal structure of MgB_{2} is very simple. It is composed of layers of boron and magnesium, alternating along the c-axis. Each boron layer has a hexagonal lattice similar to that of graphite. The magnesium atoms are arranged between the boron layers in the centers of the hexagons. This has allowed to perform consistent calculations of its electronic structure. Band structure calculations of MgB_{2} show that there are at least two types of nearly separated bands with two superconducting gaps in the excitation spectrum at the Fermi surface. The first one is a heavy hole band, built up of boron σ orbitals. The second one is the broader band with a smaller effective mass, built up mainly of π boron orbitals [3-7].

It is now well established that MgB_{2} is an anisotropic two-gap superconductor [4]. The gap ratio for the larger gap is 7.6. For the smaller gap, this ratio is around 2.78, so that. Seemingly, both the energy gaps have s-wave symmetries, the larger gap is highly anisotropic, while the smaller one is either isotropic or slightly anisotropic. The induced character of manifests itself in its temperature dependence. The larger energy gap occurs in σ-orbital band, while in the π-orbital band. For a simplified description, single effective σ- and π-bands can be introduced.

The Fermi surface consists of four sheets: two three dimensional sheets form the π bonding and antibonding bands, and two nearly cylindrical sheets form the two-dimensional σ-band [4,8]. There is a large difference in the electron-phonon coupling on different Fermi surface sheets and this leads to multiband description of superconductivity. The average electronphonon coupling strength is found to have small values [9-11]. Ummarino et al. [12] proposed that MgB_{2} is a weak coupling two band phononic system where the Coulomb pseudopotential and the interchannel paring mechanism are key terms to interpret the superconducting state. Garland [13] has remarked that Coulomb potential in the d-orbitals of the transition metal reduce the isotope exponent, whereas sp-metals generally shows a nearly full isotope effect. Clearly, like sp metal, for MgB_{2} the Coulomb effect cannot be considered to explain the reduction of isotope exponent.

It is quite natural to describe a two-gap superconductor by means of a two-band model with interband coupling [14,15]. For MgB_{2}, an approach of such kind is also directly proposed by the nature of the electron spectrum mentioned. There is a number of two band type approaches for superconductivity in MgB_{2} [16]. We may note that two band models have been exploited in various realizations for high-T_{c} cuprate superconductivity [16,17].

Liu et al. [4] pointed the role of the electron-phonon interaction between effective σ- and π-bands in the two gap system MgB_{2}. In the present study, we use σ-π interband coupling with a strong σ-interband contribution of electron-phonon and Coulobmic nature. Following Liu et al. [4], the interband interaction is considered to be repulsive (an advantage of two band models) corresponding to electron-electron interaction.

Using two band models, we study the basic MgB_{2} superconductivity characteristics, specific heat and density of states and compare the theoretical results qualitatively with the available experimental data.

2. The Model Hamiltonian

The model Hamiltonian has the form [18]

(1)

where

(2)

(3)

and

(4)

Here p and d are momentum labels in the π- and σ- bands respectively with energies and, μ is the common chemical potential. Each band has its proper pairing interaction and, while the pair interchange between the two bands is assured by term.

We have assumed, and we define the following quantities

Further we define

(5)

Now in Equation (1) read as

Final Hamiltonian can be written as

(6)

We study the Hamiltonian (6) with the Green’s function technique and equation of motion method.

2.1. Green’s Functions

In order to study the physical properties, we define the following normal and anomalous Green’s functions [18- 28]:

(7)

Following equation of motion method, we obtain Green’s functions as follows. In obtaining Green’s functions, we have assumed

and

and

Then

(8)

1) Green’s functions for π-band

(9)

(10)

2) Green’s functions for σ-band

(11)

(12)

2.2. The Correlation Functions

Using the following relation [23-27],

(13)

and employing the following identity,

we obtain the correlation functions for the Green’s functions given by Equations (9) and (10) as:

(14)

(15)

where

(16)

and are Fermi functions.

Similarly correlation functions for Green’s functions (11) and (12) for σ holes are obtained.

One can define the two superconducting order parameters related to the correlation functions corresponding to Green’s functions and for π- and σ-bands respectively. In a similar manner electronic specific heat can also be defined related to both π- and σ-bands.

3. Physical Properties

3.1. Superconducting Order Parameters

Gap parameter is the superconducting order parameter, which can be determined self consistently from the gap equations

(17)

(18)

In a matrix form, the order parameter for the superconducting state is given by [19]

(19)

where is the pairing interaction constant and function G’s are defined as

(20)

(21)

Here and are density of states for π- and σ-bands respectively at the Fermi level.

There are two superconducting gaps corresponding to π- and σ-bands in this interband model. One can write the equations for superconducting gaps corresponding to π- and σ-bands as follows

(22)

(23)

where and is pairing interaction for π- and σ- bands respectively, while the pair interchange between the two bands is assured by the term. The quantity has been supposed to be operative and constant in the energy interval for higher band and lower band, keeping in mind the integration ranges, the gap parameter satisfy the system if the interband interactions are missing, i.e., the transition is solely induced by the interband interaction [16] and given by

(24)

Using Equations (24), we can write the simultaneous equation as

(25)

(26)

3.2. Electronic Specific Heat (C_{es})

The electronic specific heat per atom of a superconductor is determined from the following relation [3,23-28]1) For π-band

(27)

where is the energy of π-band and μ is the common chemical potential.

Substituting from (10) and changing the summation over p into an integration by using the relation, we obtain

(28)

where and are given by Equation (16).

2) For σ-band Similarly one can write the expression for electronic specific heat for σ-band, as

(29)

where and are

Electronics specific heat for π-band and σ-band are given by Equations (28) and (29) respectively.

3.3. Density of States N (ω)

The density of states is an important function. This helps in the interpretation of several experimental data e.g. many processes that could occur in crystal but are forbidden because they do not conserve energy. Some of them nevertheless take place, if it is possible to correct the energy imbalance by phonon-assisted processes, which will be proportional to [25]. For, the density of states per atom is defined as [26,27].

(30)

where, is the density of state function for π- band. For σ-band we have

(31)

where is one particle Green function for π- and σ-bands, defined by Equations (9) and (11) respectively. We have the Green’s function Equation (9),

(32)

where. Now solving Equation (32) and using partial fraction method, we obtain

(33)

Now substituting the Green function from Equation (33) in Equation (30) and using the delta function property,

we obtain

(34)

Changing the summation into integration and after simplification, one obtains

(35)

Similarly, for σ-band

(36)

4. Numerical Calculations

Values of various parameters appearing in equations obtained in the previous section are given in Table 1. Using these values, we study the various parameters for the system MgB_{2}.

4.1. Superconducting Order Parameter

For the study of superconducting order parameter for MgB_{2} system within two band models, one finds the following situations1) The SC order parameter for π- and σ-bands. Using Equation (25), one can write

and

Changing the variables as, , and taking, we obtain Solving Equation (37) numerically, one can study the variation of superconductivity order parameters and with temperature corresponding π- and σ-bands. The behavior of superconducting order parameters corresponding to π- and σ-bands with temperature is shown in Figure 1.

2) SC order parameter in the presence of both π- and σ-bands.

The superconducting order parameter for combined π- and σ-bands can be studied by taking a simple sum of both the parameters. Taking the sum of order parameters, one can obtain the values by solving numerically. A comparison of with BCS type curve is shown in Figure 2.

4.2. Electronic Specific Heat (C_{es})

1) For π-band Using Equation (28) and putting a_{1}, a_{2} and, after simplification, we obtain

(38)

Changing the variables as, , and using parameters from Table 1 with taking, we obtain

(39)

2) For σ-band Similarly, we can write expression for specific heat for σ-band using Equation (29)

(37)

Table 1. Values of various parameters for MgB_{2} system.

Figure 1. Variation of superconducting order parameter corresponding to π- and σ-bands with temperature [29].

Figure 2. Variation of superconducting order parameter Δ = (Δ_{π} + Δ_{σ}) corresponding to π- and σ-bands with temperature.

(40)

The variation electronic specific heat (C_{es}) with temperature (T) for π- and σ-band is shown in Figure 3. There is a good agreement with experiment data.

4.3. Density of States

Density of states function for the π-band is given by Equation (35). Now using the following values of y, x_{1} for and x_{2} for, and taking, one obtains,

(41)

Similarly, using Equation (36), density of states for σ- band is obtained as

(42)

The above two expressions of density of states function for π- and σ-bands are similar, hence we have evaluated the values with different values of x_{1} and x_{2} for π- and σ-bands. The behavior of density of states function for both π- and σ-bands is shown in Figure 4.

5. Discussion and Conclusions

NOTES

Conflicts of Interest

The authors declare no conflicts of interest.

[1] | J. Nagamatsu, N. Nakagawa, T. Muranaka, Y. Zenitani, J. Akimitsu, “Superconductivity at 39 K in Magnesium Diboride,” Nature, Vol. 410, No. 6824, 2001, pp. 63-64. doi:10.1038/35065039 |

[2] | C. Buzea and T. Yamashita, “Review of the superconducting properties of MgB2,” Superconductor Science and Technology, Vol. 14, No. 11. 2001, p. R115. |

[3] | S. L. Kakani, S. Kakani, “Superconductivity,” Anshan, Ltd., Kent, 2009. |

[4] | A. Y. Liu, I. I. Mazin and J. Kortus, “Beyond Eliashberg Superconductivity in MgB2: Anharmonicity, Two-Phonon Scattering, and Multiple Gaps,” Physical Review Letters, Vol. 87, No. 8, 2001, pp. 087005-087009. doi:10.1103/PhysRevLett.87.087005 |

[5] | J. M. An and W. E. Pickett, “Superconductivity of MgB2: Covalent Bonds Driven Metallic,” Physical Review Letters, Vol. 86, No. 19, 2001, pp. 4366-4369. doi:10.1103/PhysRevLett.86.4366 |

[6] | K. D. Belaschenko, M. von Schilfgaarde and A. V. Antropov, “Coexistence of Covalent and Metallic Bonding in the Boron Intercalation Superconductor MgB2,” Physical Review B, Vol. 64, No. 9, 2001, pp. 092503-092507. doi:10.1103/PhysRevB.64.092503 |

[7] | D. A. Papaconstantopoulos and M. J. Mehl, “Precise TightBinding Description of the Band Structure of MgB2,” Physical Review B, Vol. 64, No. 17, 2001, pp. 2510-2514 |

[8] | I. I. Mazin and V. P. Antropo, “Electronic Structure, Electron-Phonon Coupling, and Multiband Effects in MgB2,” Physica C: Superconductivity, Vol. 385, No. 1-2, 2003, pp. 49-65. doi:10.1016/S0921-4534(02)02299-2 |

[9] | F. Bouqut, Y. Wang, R. A. Fisher, D. G. Hinks, J. D. Jorgensen, A. Junod and N. E. Phillips, “Phenomenological Two-Gap Model for the Specific Heat of MgB2,” Europhysics Letters, Vol. 56, No. 6, 2001, p. 856. doi:10.1209/epl/i2001-00598-7 |

[10] | F. Bouquet, R. A. Fisher, N. E. Phillips, D. G. Hinks and D. Jorgensen, “Specific Heat of Mg11B2: Evidence for a Second Energy Gap,” Physical Review Letters, Vol. 87, No. 4, 2001, pp. 047001-047005. doi:10.1103/PhysRevLett.87.047001 |

[11] | Y. Wang, T. Plackowski and A. Junod, “Specific Heat in the Superconducting and Normal State (2-300 K, 0-16 T), and Magnetic Susceptibility of the 38 K Superconductor MgB2: Evidence for a Multicomponent Gap,” Physica C: Superconductivity, Vol. 355, No. 3-4, 2001, pp. 179-193. doi:10.1016/S0921-4534(01)00617-7 |

[12] | G. A. Ummarino, R. S. Gonnelli, S. Massidda and A. Bianconi, “Electron-Phonon Coupling and Two-Band Superconductivity of Aland C-Doped MgB2,” 2010. |

[13] | S. L. Bud’ko, G. Lapertot, C. Petrovic, C. E. Cunningham, N. Anderson and P. C. Canfield, “Boron Isotope Effect in Superconducting MgB2,” Physical Review Letters, Vol. 86, No. 9, 2001, pp. 1877-1880. doi:10.1103/PhysRevLett.86.1877 |

[14] | H. Shul, B. T. Matthias and L. R. Walker, “Bardeen-Cooper-Schrieffer Theory of Superconductivity in the Case of Overlapping Bands,” Physical Review Letters, Vol. 3, No. 12, 1959, pp. 552-554. doi:10.1103/PhysRevLett.3.552 |

[15] | V. A. Moskalenko, M. E. Palistrant and V. M. Vakalyuk, “High-Temperature Superconductivity and the Characteristics of the Electronic Energy Spectrum,” Soviet Physics Uspekhi, Vol. 34, No. 8, 1991, p. 717. doi:10.1070/PU1991v034n08ABEH002466 |

[16] | N. Kristoffel, P. Konsin and T. Ord, “Two-Band Model for High-Temperature Superconductivity,” Rivista Del Nuovo Cimento, Vol. 17, No. 9, 1994, pp. 1-41. doi:10.1007/BF02724515 |

[17] | N. Kristoffel and P. Rubin, “Pseudogap and Superconductivity Gaps in a Two Band Model with Doping Determined Components,” Solid State Communications, Vol. 122, No. 5, 2002, pp. 265-268. |

[18] | B. K. Chakraverty, “Superconductivity in Two Band Model,” Physical Review B, Vol. 48, No. 6, 1993, pp. 4047-4053. doi:10.1103/PhysRevB.48.4047 |

[19] | R. Lal, Ajay, R. L. Hota and S. K. Joshi, “Model for c-Axis Resistivity of Cuprate Superconductors,” Physical Review B, Vol. 57, No. 10, 1998, pp. 6126-6136. doi:10.1103/PhysRevB.57.6126 |

[20] | A. Pratap, Ajay and A. S. Tripathi, “Effect of Interlayer Interactions in High-Tc Cuprate Supercoductors,” Journal of Superconductivity, Vol. 9, No. 6, 1996, pp. 595-597. doi:10.1007/BF00728239 |

[21] | S. Khandka and P. Singh, “Effect of Interlayer Interaction on Tc with Number of Layers in High Tc Cuprate Superconductors,” Physica Status Solidi B, Vol. 244, No. 2, 2007, pp. 699-708. doi:10.1002/pssb.200542285 |

[22] | S. Das and N. C. Das, “ Erratum: Theory of Hole Superconductivity,” Physical Review B, Vol. 46, No. 10, 1992, pp. 6451-6457. doi:10.1103/PhysRevB.46.6451 |

[23] | S. L. Kakani and U. N. Upadhyaya, “Cooperative Phenomena in Ternary Superconductors,” Journal of Low Temperature Physics, Vol. 53, No. 1-2, 1983, pp. 221-253. doi:10.1007/BF00685781 |

[24] | S. L. Kakani and U. N. Upadhyaya, “Superconducting and Magnetic Order Parameters in the Coexistence Region of Ternary Superconductors,” Physica Status Solidi B, Vol. 125, No. 2, 1984, pp. 861-867. doi:10.1002/pssb.2221250249 |

[25] | S. L. Kakani and U. N. Upadhyaya, “Frequency Dependent Susceptibility of Rare Earth Ternary Superconductors,” Physica Status Solidi B, Vol. 136, No. 1, 1986, pp. 115-121. doi:10.1002/pssb.2221360113 |

[26] | S. L. Kakani and U. N. Upadhyaya, “Coexistence of Superconductivity and Ferromagnetism in Rare Earth Ternary Systems,” Physica Status Solidi A, Vol. 99, No. 1, 1987, pp. 15-36. doi:10.1002/pssa.2210990104 |

[27] | S. L. Kakani and U. N. Upadhyaya, “Magnetic Superconductors: A Review,” Journal of Low Temperature Physics, Vol. 70, No. 1-2, 1988, pp. 5-82. doi:10.1007/BF00683246 |

[28] | A. L. Fetter and J. D. Walecka, “Quantum Theory of Many Particle Physics,” McGraw-Hill, New York, 1971. |

[29] | C. Buzea and T. Yamashita, “Review of the Superconducting Properties of MgB2,” Superconductor Science and Technology, Vol. 14, No. 11, 2001, p. R115. doi:10.1088/0953-2048/14/11/201 |

[30] | C. Walti, E. Felder, C. Degen, G. Wigger, R. Monnier, B. Delley and H. R. Ott, “Strong Electron-Phonon Coupling in Superconducting MgB2: A Specific Heat Study,” Physical Review B, Vol. 64, No. 17, 2001, pp. 172515172519. doi:10.1103/PhysRevB.64.172515 |

[31] | N. E. Phillips and R. A. Fisher, “Superconducting-State Energy Gap Parameters from Specific Heat Measurements,” Journal of Thermal Analysis and Calorimetry, Vol. 81, No. 3, 2005, pp. 631-635. doi:10.1007/s10973-005-0835-y |

[32] | S. L. Kakani, “Superconductivity: Current Topics: Chapters 2 and 3,” Bookman Associate, Jaipur, 1999. |

[33] | S. Kakani and S. L. Kakani, “Theoretical Study of Specific Heat, Density of States and Free Energy of Itinerant Ferromagnetic Superconductor URhGe,” Journal of Superconductivity and Novel Magnetism, Vol. 22, No. 7, 2009, pp. 677-685. doi:10.1007/s10948-009-0465-x |

[34] | A. Kashyap, S. C. Tiwari, A. Surana, R. K. Paliwal and S. L. Kakani, “Theoretical Study of Specific Heat, Density of States, Free Energy,and Critical Field of High Temperature Cuprate Superconductors Based on Intra and Interlayer Interactions,” Journal of Superconductivity and Novel Magnetism, Vol. 21, No. 2, 2008, pp. 129-143. doi:10.1007/s10948-008-0308-1 |

[35] | A. Nuwal, R. K. Paliwal, S. L. Kakani and M. L. Kalara, “Theoretical study of Photoinduced Superconductors in a Two Band Model,” Physica C: Superconductivity, Vol. 471, No. 9-10, 2011, pp. 318-331. doi:10.1016/j.physc.2011.03.004 |

[36] | G. Alecu, “Reports in Physics,” Romanian Reports in Physics, Vol. 56, No. 3, 2004, pp. 404-412. |

Journals Menu

Contact us

+1 323-425-8868 | |

customer@scirp.org | |

+86 18163351462(WhatsApp) | |

1655362766 | |

Paper Publishing WeChat |

Copyright © 2024 by authors and Scientific Research Publishing Inc.

This work and the related PDF file are licensed under a Creative Commons Attribution 4.0 International License.